BUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION


 Wilfred Cooper
 1 years ago
 Views:
Transcription
1 2 th International Conference on Composite Materials Copenhagen, th July 215 BUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION José Humberto S. Almeida Jr. 1, Marcelo L. Ribeiro 2, Volnei Tita 2, Hugo Faria 3, António T. Marques 4, Sandro C. Amico 1 1 PPGE3M, Federal University of Rio Grande do Sul, Av. Bento Gonçalves, Porto Alegre, RS, Brazil 2 Department of Aeronautical Engineering, Engineering School of São Carlos, University of São Paulo, Av. João Dagnone 11, São Carlos, SP, Brazil 3 Composite Materials Unit, INEGI  Institute of Mechanical Engineering and Industrial Management, Rua Dr. Roberto Frias 4, , Porto, Portugal 4 FEUP  Faculty of Engineering of the University of Porto, Rua Dr. Roberto Frias s/n, , Porto, Portugal Keywords: buckling, composite tubes, filament winding, postbuckling, progressive failure ABSTRACT Transverse compression (ring deflection) tests were simulated in composite tubes through nonlinear finite element models based on a modified Riks algorithm, which uses the arclength method. Progressive failure was evaluated in detail through a proposed damage model, able to identify the failure mode. In all composite tubes tested, localized stress concentration points developed in the transverse plane caused by contact load plates/composite, producing nonlinearity in the load vs. displacement curves (P ). The failure mode of these tubes involves a complex combination of mechanisms, namely transverse tensile, transverse compression and inplane shear stresses, where the region of the specimen in contact with the load plates present the most damaged area. Thus, matrix tensile and matrix compression induced by shear near the loading zones dominate damage and failure of the specimens. Buckling and postbuckling of tubes are highly influenced by the fiber orientation, whereas the tube with reinforcement orientation parallel to the loading platestospecimens contact line withstanding the highest buckling load level. On the other hand, specimens wound at [±45] 5 and [±75] 5 present a divergence point, since they support a portion of the load after buckling is reached, characterizing a postbuckling behavior. 1 INTRODUCTION Cylindrical shells have numerous applications in aerospace, aeronautic and marine structures, such as in launch vehicle fuel tanks, fuselages and offshore structures. They have the ability to carry high levels of axial and transverse compression, since most of the structure is loaded in a membrane state and its efficiency is derived from the lack of throughthethickness stress gradients [1]. These structures are traditionally metallicbased, therefore due to the evergrowing need to decrease the payload in such aeronautic and marine structures, the use of polymeric composites is being motivated, mainly due to their high corrosion resistance and high stiffness and strengthtoweight ratios. Filament winding (FW) process stands out in composite materials processing because of its high precision in fiber positioning, high fiber content, high automation capability and low void content. Due to these characteristics, FW is the most common process for manufacturing revolution and axisymmetric parts, such as composite overwrapped pressure vessels and tubes. When these structures
2 José Humberto S. Almeida Jr., Marcelo L. Ribeiro, Volnei Tita, Hugo Faria, António T. Marques, Sandro C. Amico act under uniaxial or biaxial load, as the load increases steadily, the shell starts to deform stably. When the load achieves a critical point, the equilibrium stops and instability may be set. Thus, buckling occurs when the structure suddenly deflects unstably and loses its capacity to keep resisting the compressive loading. Fig. 1 shows a typical load vs. displacement response for an unstable problem. Composite tubes with a sufficiently thinwall shell fail due to either global or local buckling when under an instable loading, and they have two possible distinct characteristics: the first one is that the development of significant radial and/or axial displacements is followed by the development of global buckling phenomena and a consequently collapse; and the second one is that the prediction of the load level at which collapse occurs is difficult when compared to wellbehaved structures, such as beams and plates [1,2]. Figure 1: Typical response of a structure under unstable loading [3]. It is common to find researches dealing with isotropic and even composite tubes under axial compression [4,5,6], which is the most classical case of a structure under an instable loading that causes buckling. However, there are no reports about the buckling behavior of composite cylindrical shells under transverse compression, which can be relevant for tubes acting under either transverse compression or hydrostatic external pressure. In both cases, the structure can fail by buckling or material failure, where they are strongly dependent of the stacking sequence, wall thickness, boundary conditions or geometrical imperfections [7]. In some cases, the structure can support a portion of the applied loading after buckling is reached, formerly known as postbuckling, typical of isotropic metallic structures. However, a composite structure may also present a postbuckling behavior even with its brittle fracture behavior. For instance, White et al. [1] performed the postbuckling analysis of variablestiffness cylindrical shells under axial compression through linear and nonlinear analysis, where both presented results within the error range achieved in experimental results, but the nonlinear analysis predicted better the final postbuckled shape. Tafreshi [2] developed a numerical model to predict the buckling and postbuckling behavior of composite cylinders under external pressure and axial compression, where the delamination was the main cause of the buckling. Harte and Fleck [8] investigated the failure behavior of braided composite cylinders under axial compression and torsion, where different failure modes were successfully predicted in the developed models. In this context, this work deals with the development of reliable models to represent the buckling and postbuckling behavior of composite tubes under transverse compression (also referred to as ring deflection). Two strategies have been implemented: i) geometrically nonlinear analyses and ii) advanced damage modelling. 2 BASICS OF BUCKLING 2.1 Linear buckling analysis Firstly, a linear Eigenvalue buckling analysis was carried out aiming at determining the buckling
3 2 th International Conference on Composite Materials Copenhagen, th July 215 critical load and the deformed shape for the composite tubes under transverse compression. The essence of an eigenvalue buckling problem is to find the loads where the stiffness matrix becomes singular, and thus the problem has nontrivial solutions [9], being represented by Eq. 1: K mn υ m = (1) where K mn is the tangent stiffness matrix when the load is applied and υ m are nontrivial displacement solutions. In the linear buckling analysis, a perturbation is applied to the undeformed shape of the specimen. Specified sets of loadings are monitored for which deflections could induce instability when under a geometric nonlinearity (also known as PDelta, P, effect), which involves the equilibrium and compatibility relationships of a structural system loaded about its deflected configuration [3]. Linear buckling procedure generates a range of buckling factors and corresponding mode shapes. When loading is multiplied by these buckling factors, the resulting scaled loading conditions represent those that induce buckling. Similarly, the mode shapes are normalized displacement sets which indicate the configuration of the buckled structure [1,11]. 2.2 Nonlinear buckling and postbuckling analysis In order to evaluate both buckling and postbuckling of the structure, a nonlinear buckling model is suitable to provide more accurate results than the elastic formulation. In this analysis, an applied loading incrementally increases until a large change in displacement occurs for a certain increment. This condition typically points that the structure has become unstable. Nonlinear buckling analysis is a static method that accounts for material and geometric nonlinearity, load perturbations and/or geometric imperfections. Geometrically nonlinear static problems occasionally involve buckling or collapse behavior, where the loaddisplacement response displays a negative stiffness and the structure should release strain energy to remain in equilibrium [2]. Buckling analysis commonly provides a bifurcation after the structure loses its equilibrium, but even in snapthrough problems (equilibrium path in loaddisplacement space is smoothed and does not branch) the Riks algorithm may be employed. In case of a snapthrough behavior, the structure can carry increasing load after a complete snap [12]. 3 MATERIAL MODEL This material model was originally developed by Ribeiro et al. [7] at a mesoscale approach, where it was adapted to the material and geometry herein used. The model regards to the composite lamina under plane stress state and the damage is considered uniform throughout the laminate thickness [13]. 3.1 Fiber modelling A unidirectional carbon/epoxy composite laminate under tensile loading in the fiber direction (σ 11 ) is linear elastic with brittle fracture. Thus, for tensile load in fiber direction, the maximum stress criterion is used to identify the fiber failure: σ 11 X t 1 (1) After failure is reached, the damage variable in fiber direction (d 1 ) is set to.99. There is no evolution of d 1 aiming at represent the catastrophic failure of the carbon fiber. To avoid possible localization issues, the degradation of properties is calculated in the step i, however it is applied into the step i + 1, thus improving the convergence process. The fiber behavior under compressive longitudinal load is set to be linear elastic until a specified value, after that, a nonlinear elastic behavior is observed. The linear elastic to nonlinear elastic limit (X C ) is then used in Eq. 2 to represent the compressive failure, as follows: σ 11 X C 1 (2) After σ 11 X C any increase in the compression loads in fiber direction results in a nonlinear
4 José Humberto S. Almeida Jr., Marcelo L. Ribeiro, Volnei Tita, Hugo Faria, António T. Marques, Sandro C. Amico elastic stress strain behavior. This nonlinear elastic behavior is simulated using a secant modulus as can be seen in Eq. 3: E 11 = X C ε 11 (1 h(ε 11)) + h(ε 11 )E 11 (3) Where h(ε 11 ) is obtained from the fit of stressstrain plots for specimens under compressive loading, ε 11 is the strain in longitudinal direction and E 11 is the initial elastic modulus from specimens under compression loading. 3.2 Matrix modelling In a unidirectional quasiflat filament wound laminate, the damage process in the matrix is essentially dominated by the transverse loading (σ 22 ) and shear loading (τ 12 ). A nonlinear behavior in the matrix is reported due to inelastic strains and damage in matrix [14]. To model the damage process in matrix, two internal damage variables, d 2 (related to σ 22 ) and d 6 (related to τ 12 ), were used. Based on Continuous Damage Mechanics, the hypothesis of effective stress links the damage variables to the stresses [9], and Eq. 4 gives the relationship σ 11 { σ 22 } = τ 12 [ 1 1 d1 1 1 d2 1 1 d6 ] σ 11 { σ 22 } (4) τ 12 where σ ij τ ij are the second order effective stress tensors. According to Herakovich [9], the damage strain energy density can be described in function of effective stresses considering only for matrix phase stresses, as shows Eq. (5) E D = 1 [ σ σ 22 2 E 22 (1 d 2) E 22 + τ 12 2 ] (5) G 12 (1 d 6 ) where σ = σ 22 if σ 2 22 >, otherwise σ = if σ 2 22 <. Similarly, σ = σ 22 if σ 2 22 <, otherwise σ 2 22 = if σ 2 22 >. Another aspect of the present model must be highlighted, which consists in an adjustment of the Poisson s coefficient for consider the damage effect. Using CDM formulation performed by Matzenmiller et al. [15], Eq. 8 gives the compliance tensor: D = 1 K [ (1 d 1 )E 11 (1 d 1 )(1 d 2 )ν 21 E 22 (1 d 1 )(1 d 2 )ν 12 E 11 (1 d 2 )E 22 K(1 d 6 )G 12 ] (8) where, K = (1 (1 d 1 )(1 d 2 )ν 12 ν 21. Aiming at avoiding the material selfhealing, the damage parameters (d 1, d 2 e d 6 ) are assumed as the maximum.99 along the simulation [7]. 4 FINITE ELEMENT MODELLING The herein presented models were built up in Abaqus 6.14 software platform. The original dimensions of the tubes are: length (l) = 381 mm, radius (r) = 68 mm and lamina thickness (t l ).6 mm (t l varies according to winding angle). The structure was modeled with S4R shell elements with three integration points in each layer. The cylindrical shell has been submitted to a transverse compressive load by contact from the compression plates (rigid bodies). Fig. 3 depicts the assembly of the virtual test. The tubes were modelled by using four node reduced integration shell element (S4R) with hourglass control. Table 1 presents the comprehensive material properties of the carbon/epoxy laminates. A compressive load was applied into the top compressive plate (rigid body) and the other plate is clamped. The buckling loading was transmitted to the specimen by contact from the rigid bodies. A modified Riks algorithm based on the arclength method was used to predict is buckling and/or postbuckling occurs. Figure 2 presents the assembly of the virtual test.
5 2 th International Conference on Composite Materials Copenhagen, th July 215 Elastic constants Strengths E 1 (GPa) E 2 = E 3 (GPa) G 12 = G 13 (GPa) 5.44 G 23 (GPa) 2.1 X t (MPa) X c (MPa) 74. Y t (MPa) 42.5 Y c (MPa) 14.3 S 12 (MPa) 68.9 Table 1: Material properties used as input in the numerical models. 4.1 Parametric study Figure 2: Assembly of the transverse compression test. A parametric study was carried out aiming at evaluate the mechanical response of the tube with different winding sequence and radius/thickness (r/t) ratios. Table 1 shows all configurations used in the simulations. Specimen code Stacking sequence r/t ratio [±45] 5 [±45] 5 [±75] 5 [±75] [±9] 5 [9] 5 r/t_22.7 [9] r/t_28.3 [9] r/t_37.7 [9] Table 2: Description of all specimen configurations used for the parametric study. 5 RESULTS AND DISCUSSION Figure 3 presents the linearelastic simulations to identify the global mechanical response of the tubes with different winding angles under transverse compression. The tube wound with hoop layers ([9] 5 ) supports higher compressive load than the other layups simulated. This performance was foreseen since the composite tube is loaded in fiber (hoop) direction. Even with geometric nonlinearity activated in the model, it is obvious that no buckling happens, where all specimens supported the
6 Load proportionality factor Load (N) José Humberto S. Almeida Jr., Marcelo L. Ribeiro, Volnei Tita, Hugo Faria, António T. Marques, Sandro C. Amico applied load until the maximum displacement set. Displacement (mm) [±45]5 [±75]5 [±9]56 Figure 3: Load displacement curves for the three winding angle evaluated through a nonlinear elastic analysis with geometric nonlinearity activated. Figure 4 shows the load proportionality factor (LPF) vs. total arc length of the simulations through a nodal analysis, aiming at finding the bifurcation point and critical buckling load for the tubes analyzed. In these plots, the values are not relevant, however the curve shape reveals the geometrical instability throughout the analysis. As can be noted, the fiber orientation influences directly on the compressive behavior of composite tubes, since the specimen [9] 5 present a clear buckling load without evidence of postbuckling, considering that when the structure buckles the analysis converges to a unique solution, a failure by buckling. On the other hand, the specimens [±45] 5 and [±75] 5 do not present a clear buckling load, but it is possible to find a bifurcation point due to the nonlinear shape of the curves. Arc length [±45]5 [±75]5 [±9]52.5 Figure 4: Load proportionality factor vs. arc length obtained from the nodal analysis for identify the buckling load and bifurcation point. Figure 5 may complement previous results obtained from Figure 4, showing the load vs. displacement plots for the cylinders. Specimen [±45] 5 presents a slightly drop at around 2 kn with a displacement of 4 mm, which can be find as a bifurcation point, to be confirmed by analyzing the material failure. The cylinder wound at [±75] 5 is the sequence that presents less influence of buckling,
7 Load (N) 2 th International Conference on Composite Materials Copenhagen, th July 215 since the cylinder start to behave slightly instable after a displacement of 3 mm. The specimen [9] 5 loses its structural integrity at 44.7 kn, being that the buckling load. Displacement (mm) [±45]5 [±75]5 [±9] Figure 5: Load displacement profile curves for the tubes with different winding angle through a nodal analysis. Analyzing the shape of the cylinders in an increment that the structure starts to lose structural stability (Figure 6), it is clear that the tubes are too dependent of the fiber orientation, since the hoop wound tube presents a typical mode I of buckling under a compressive load. However, it cannot be stated that any of these structures may failed buckling. For that, a failure evaluation seems crucial to understand the complete behavior of these structures under an unstable load. Figure 6: Deformed shape of the tubes at the increment in which the structure starts to be unstable. 5.1 Failure and damage analysis Figure 7 presents the progressive failure analysis for the tubes exhibited through the load vs. displacement curves. As can be noted, the tube [9] 5 presented a sudden failure at 25 kn with a displacement 2.7 mm. Although Riks analysis pointed a buckling load of 44.7 kn, the failure analysis evidences that the tube fails by material failure before achieve the buckling load. The specimen [±45] 5 has a bifurcation point at a load of 18.1 kn at the displacement of 38.2 mm, which is similar to buckling load found at the nodal analysis. This curve shape suggests a postbuckling behavior, since the specimen does not fail at the buckling load, since the structure keep carrying a portion of the compressive load. The tube [±75] 5 points a bifurcation at a load of 24.5 kn and displacement of 35.7 mm, but with a large amount of failed plies, characterizing that the structure postbuckles but with various plies damaged. It is interesting to observed in these load vs. displacement profiles that the curves fluctuate along the analysis with several tiny discontinuities, which may correspond to progressive failure of the plies. A typical issue in these test is the contact between the rigid plates and the composite specimen, since
8 Load (N) Load (N) José Humberto S. Almeida Jr., Marcelo L. Ribeiro, Volnei Tita, Hugo Faria, António T. Marques, Sandro C. Amico this contact may induce a transverse shear between them, being cause a premature failure of the specimen. Displacement (mm) First matrixdominated ply failed Ultimate and fiberdominated failure 51 Matrixdominated elements failed Bifurcation point [±45]5 [±75]5 [±9]5 Material failure 3 Figure 7: Mechanical response of the tubes simulated by using the damage model herein proposed. It is observed a high dependence of the winding angle on the failure of the specimens under the compressive load. As the winding angle increases, the failure load increases. The analysis indicate that when the fiber orientation is aligned perpendicular to the loading axis, the cylinder become more stable under transversal compressive loading. Thus, with fibers wound in the hoop direction, the tube is more able to sustain higher hoop stress levels prior to failure. 5.2 Parametric study Figure 7 shows typical curves for the tube [9] 5 with different radiustothickness (r/t) ratios. As the r/t ratio increase, the buckling load decreases, once as thinner as the wall thickness the structure becomes more susceptible to buckling. In addition, as higher as the r/t ratio, the specimen displace more at a lower maximum peak load. The specimen r/t_37.7 has the most instability throughout the analysis, which can be attributed to the high influence of transverse shear stresses. Despite at different loads, a similar profile is observed for each tube until 2 mm, presenting a linear response. The deviation from linearity to nonlinearity is clear for all specimens, even though at different load stages indicating active damage mechanisms in all tubes r/t_22.7 r/t_ Displacement (mm) 3 Figure 8: Mechanical response for the cylinders with several radiustothickness ratios.
9 2 th International Conference on Composite Materials Copenhagen, th July 215 The deformed shape of these tubes at the failure load is shown in Figure 9, where the thinnest tube present a bifurcation point at a load of 7.8 kn and a displacement of 25 mm, being this the reason for a high displacement by supporting a small portion of the load (compared to the other tubes). This cylinder has a matrixdominated failure mode, mainly by transverse shear and transverse tensile stresses. It is valid to mention the stress concentrations created at the contact plate/specimen, however this cylinder does not present fiberdominated failure. Figure 9: Final deformed shape of each tube and their spatial displacement in the circumferential direction. 6 CONCLUSIONS The scope of this paper was to evaluate the buckling and/or postbuckling response of filament wound composite tubes under a transversal compressive load. For that, a nonlinear analysis based on a modified arclength method was used to predict the buckling load and the bifurcation point. In addition, a damage model was proposed, in order to understand the progressive failure and damage upon buckling onset of the tubes with several winding angle and radiustothickness ratio. The specimen wound with hoop layers supported the highest compressive load, pointing a buckling load of about 4 kn, whereas the tubes [±45] 5 and [±75] 5 have a bifurcation point in lower loads, presenting a postbuckling behavior, since the structure still support portion of the load of buckling is reached. However, the specimen [9] 5 failed in the material before a buckling load, with a combination of transverse tensile, inplane shear and radial compression, beyond a few fiberdominated failures at the contact between the rigid plates and composite specimen, being this point the final failure location. The failure analysis corroborated that the [±45] 5 and [±75] 5 present postbuckling after a displacement at around 4 mm, and the tube [9] 5 did not show postbuckling. The next step of this research is to carry out the experiments to validate the buckling and postbuckling models herein developed, as well as the damage model and progressive failure of the plies during this test. ACKNOWLEDGEMENTS The authors are grateful to CAPES, CNPq, AEB (Brazilian Space Agency) and CCDRN (Portugal) for the financial support to this study, through corresponding cofunded programs. REFERENCES [1] S.C. White, P.P. Weaver, K.C. Wu, Postbuckling analyses of variablestiffness composite cylinders in axial compression, Composite Structures, 123, 215, pp (doi: 1.116/j.compstruct ). [2] A. Tafreshi, Delamination buckling and postbuckling in composite cylindrical shells under combined axial compression and external pressure, Composite Structures, 72(4), 26, pp (doi: 1.116/j.compstruct ).
10 José Humberto S. Almeida Jr., Marcelo L. Ribeiro, Volnei Tita, Hugo Faria, António T. Marques, Sandro C. Amico [3] Dassault Systèmes Simulia Corporation, Abaqus 6.13, Analysis User's Guide, Providence, RI, USA, 214. [4] A. Tafreshi, Efficient modelling of delamination buckling in composite cylindrical shells under axial compression, Composite Structures, 64(34), 24, pp (doi: 1.116/j.compstruct ). [5] C. Bisagni and P. Cordisco, An experimental investigation into the buckling and postbuckling of CFRP shells under combined axial and torsion loading, Composite Structures, 6(4), 23, pp (doi: 1.116/S (3)242). [6] T. von Kármán and HS. Tsien, The Buckling of Thin Cylindrical Shells under Axial Compression, Journal of Spacecraft and Rockets, 4(6), 23, pp (doi: /2.756). [7] M. Życzkowsky, Postbuckling analysis of nonprismatic columns under general behaviour of loading, International Journal of NonLinear Mechanics, 4(4), 25, pp (doi: 1.116/j.ijnonlinmec ). [8] AM. Harte and N.A. Fleck, Deformation and failure mechanisms of braided composite tubes in compression and torsion, Acta Materialia, 48(6), 2, pp (doi: 1.116/S (99)4279). [9] S. Novoselac, T. Ergić, P. Baličević, Linear and nonlinear buckling and post buckling analysis of a bar with the influence of imperfections, Tehnički Vjesnik, 19(3), 212, pp [1] M.W. Hilburger and J.H. Starnes Jr, Effects of imperfections on the buckling response of compressionloaded composite shells, International Journal of NonLinear Mechanics, 37(45), 22, pp (doi: 1.116/S27462(1)889). [11] V.V. Bolotin, Delamination in composite structures: its origin, buckling, growth and stability. Composites Part B, 27(2), 1996, pp (doi: 1.116/ (95)356). [12] E. Riks, An incremental approach to the solution of snapping and buckling problems, International Journal of Solids and Structures, 15(7), 1979, pp (doi: 1.116/27683(79)9817). [13] C. Herakovich, Mechanics of fibrous composites, Vol. 1, Wiley Publisher, [14] A. Puck, H. Schürmann, Failure analysis of FRP laminates by means of physically based phenomenological models, Composites Science and Technology, 58(7), 1998, pp (doi: 1.116/S (1)281). [15] A. Matzenmiller, J. Lubliner, R.L. Taylor, A constitutive model for anisotropic damage in fibercomposites, Mechanics of Materials, 2(2), 1995, pp (doi: 1.116/ (94)53).
Dynamic Response Of Laminated Composite Shells Subjected To Impulsive Loads
IOSR Journal of Mechanical and Civil Engineering (IOSRJMCE) eissn: 22781684,pISSN: 2320334X, Volume 14, Issue 3 Ver. I (May.  June. 2017), PP 108123 www.iosrjournals.org Dynamic Response Of Laminated
More informationNumerical Analysis of Composite Panels in the PostBuckling Field taking into account Progressive Failure
Copyright c 007 ICCES ICCES, vol.1, no.3, pp.9398, 007 Numerical Analysis of Composite Panels in the PostBuckling Field taking into account Progressive Failure C. Bisagni 1 Summary The research here
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationFinite Element Analyses of Low Velocity Impact on Thin Composite Disks
International Journal of Composite Materials 2013, 3(6B): 5970 DOI: 10.5923/s.cmaterials.201310.07 Finite Element Analyses of Low Velocity Impact on Thin Composite Disks Marcelo L. Ribeiro 1, Ricardo
More informationUltimate shear strength of FPSO stiffened panels after supply vessel collision
Ultimate shear strength of FPSO stiffened panels after supply vessel collision Nicolau Antonio dos Santos Rizzo PETROBRAS Rio de Janeiro Brazil Marcelo Caire SINTEF do Brasil Rio de Janeiro Brazil Carlos
More informationMulti Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala
Multi Disciplinary Delamination Studies In Frp Composites Using 3d Finite Element Analysis Mohan Rentala Abstract: FRP laminated composites have been extensively used in Aerospace and allied industries
More informationA RESEARCH ON NONLINEAR STABILITY AND FAILURE OF THIN WALLED COMPOSITE COLUMNS WITH OPEN CROSSSECTION
A RESEARCH ON NONLINEAR STABILITY AND FAILURE OF THIN WALLED COMPOSITE COLUMNS WITH OPEN CROSSSECTION H. Debski a*, J. Bienias b, P. Jakubczak b a Faculty of Mechanical Engineering, Department of Machine
More informationPREDICTION OF OUTOFPLANE FAILURE MODES IN CFRP
PREDICTION OF OUTOFPLANE FAILURE MODES IN CFRP R. R. Pinto 1, P. P. Camanho 2 1 INEGI  Instituto de Engenharia Mecanica e Gestao Industrial, Rua Dr. Roberto Frias, 4200465, Porto, Portugal 2 DEMec,
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationKINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP)
KINK BAND FORMATION OF FIBER REINFORCED POLYMER (FRP) 1 University of Science & Technology Beijing, China, niukm@ustb.edu.cn 2 Tsinghua University, Department of Engineering Mechanics, Beijing, China,
More informationREPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 REPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
More informationCrashworthy Design of Composite Structures Using CAE Process Chain
0 th European LSDYNA Conference 205, Würzburg, Germany Crashworthy Design of Composite Structures Using CAE Process Chain Madhukar Chatiri, Thorsten Schuetz 2, Anton Matzenmiller 3 CADFEM GmbH, Grafing
More informationOpenhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More informationA STRUCTURE DESIGN OF CFRP REAR PRESSURE BULKHEAD WITHOUT STIFFENERS
Xi an, 225 th August 217 A STRUCTURE DESIGN OF CFRP REAR PRESSURE BULKHEAD WITHOUT STIFFENERS LI Zhongyang 1, LI Dong 2 Mailbox7235, Yanliang District, Xian, China, Email: zhongyangli@live.com Keywords:
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationUniversity of Sheffield The development of finite elements for 3D structural analysis in fire
The development of finite elements for 3D structural analysis in fire Chaoming Yu, I. W. Burgess, Z. Huang, R. J. Plank Department of Civil and Structural Engineering StiFF 05/09/2006 3D composite structures
More informationMultiscale Approach to Damage Analysis of Laminated Composite Structures
Multiscale Approach to Damage Analysis of Laminated Composite Structures D. Ivančević and I. Smojver Department of Aeronautical Engineering, Faculty of Mechanical Engineering and Naval Architecture, University
More informationPrediction of Elastic Constants on 3D Fourdirectional Braided
Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Liang Dao Zhou 1,2,* and Zhuo Zhuang 1 1 School of Aerospace,
More informationLINEAR AND NONLINEAR BUCKLING ANALYSIS OF STIFFENED CYLINDRICAL SUBMARINE HULL
LINEAR AND NONLINEAR BUCKLING ANALYSIS OF STIFFENED CYLINDRICAL SUBMARINE HULL SREELATHA P.R * M.Tech. Student, Computer Aided Structural Engineering, M A College of Engineering, Kothamangalam 686 666,
More informationSIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS
VOL. 5, NO. 4, APRIL 010 ISSN 18196608 006010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
More informationOn Nonlinear Buckling and Collapse Analysis using Riks Method
Visit the SIMULIA Resource Center for more customer examples. On Nonlinear Buckling and Collapse Analysis using Riks Method Mingxin Zhao, Ph.D. UOP, A Honeywell Company, 50 East Algonquin Road, Des Plaines,
More informationWhat to expect when you re expecting FEA A guide to good practice
What to expect when you re expecting FEA A guide to good practice 1. Background Finite Element Analysis (FEA) has transformed design procedures for engineers. Allowing more complex geometry, loading and
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationFEA A Guide to Good Practice. What to expect when you re expecting FEA A guide to good practice
FEA A Guide to Good Practice What to expect when you re expecting FEA A guide to good practice 1. Background Finite Element Analysis (FEA) has transformed design procedures for engineers. Allowing more
More informationSamantha Ramirez, MSE. Stress. The intensity of the internal force acting on a specific plane (area) passing through a point. F 2
Samantha Ramirez, MSE Stress The intensity of the internal force acting on a specific plane (area) passing through a point. Δ ΔA Δ z Δ 1 2 ΔA Δ x Δ y ΔA is an infinitesimal size area with a uniform force
More informationEXPLICIT DYNAMIC SIMULATION OF DROPWEIGHT LOW VELOCITY IMPACT ON CARBON FIBROUS COMPOSITE PANELS
EXPLICIT DYNAMIC SIMULATION OF DROPWEIGHT LOW VELOCITY IMPACT ON CARBON FIBROUS COMPOSITE PANELS Umar Farooq and Karl Gregory School of Built Environment and Department of Engineering, University of Bolton,
More information202 Index. failure, 26 field equation, 122 force, 1
Index acceleration, 12, 161 admissible function, 155 admissible stress, 32 Airy's stress function, 122, 124 d'alembert's principle, 165, 167, 177 amplitude, 171 analogy, 76 anisotropic material, 20 aperiodic
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationAim of the study Experimental determination of mechanical parameters Local buckling (wrinkling) Failure maps Optimization of sandwich panels
METNET Workshop October 1112, 2009, Poznań, Poland Experimental and numerical analysis of sandwich metal panels Zbigniew Pozorski, Monika ChudaKowalska, Robert Studziński, Andrzej Garstecki Poznan University
More informationStresses Analysis of Petroleum Pipe Finite Element under Internal Pressure
ISSN : 4896, Vol. 6, Issue 8, ( Part 4 August 06, pp.338 RESEARCH ARTICLE Stresses Analysis of Petroleum Pipe Finite Element under Internal Pressure Dr.Ragbe.M.Abdusslam Eng. Khaled.S.Bagar ABSTRACT
More informationUnit 18 Other Issues In Buckling/Structural Instability
Unit 18 Other Issues In Buckling/Structural Instability Readings: Rivello Timoshenko Jones 14.3, 14.5, 14.6, 14.7 (read these at least, others at your leisure ) Ch. 15, Ch. 16 Theory of Elastic Stability
More informationAnalysis of Composite Pressure Vessels
Analysis of Composite Pressure Vessels Reza Mohammadzadeh Gheshlaghi 1 Mohammad Hassan Hojjati Hamid Reza Mohammadi Daniali 3 1 Engineering Research Centre, Tabriz, Iran,3 Department of Mechanical Engineering,
More informationDesign and optimization of a variable stiffness composite laminate
th World Congress on Structural and Multidisciplinary Optimisation 07 th  th, June 05, Sydney Australia Design and optimization of a variable stiffness composite laminate Yan Zhang, Fenfen Xiong Qian
More informationPROGRESSIVE DAMAGE ANALYSES OF SKIN/STRINGER DEBONDING. C. G. Dávila, P. P. Camanho, and M. F. de Moura
PROGRESSIVE DAMAGE ANALYSES OF SKIN/STRINGER DEBONDING C. G. Dávila, P. P. Camanho, and M. F. de Moura Abstract The debonding of skin/stringer constructions is analyzed using a stepbystep simulation
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationFINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Ever J. Barbero Department of Mechanical and Aerospace Engineering West Virginia University USA CRC Press Taylor &.Francis Group Boca Raton London New York
More informationPRESSURE VESSELS & PRESSURE CABINS FOR BLENDED WING BODIES
PRESSURE VESSELS & PRESSURE CABINS FOR BLENDED WING BODIES F.J.J.M.M. Geuskens, O.K. Bergsma 2, S. Koussios 2 & A. Beukers 3 PhD Researcher, 2 Associate professor, 3 Professor / DPCS, TU Delft Kluyverweg,
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationD : SOLID MECHANICS. Q. 1 Q. 9 carry one mark each. Q.1 Find the force (in kn) in the member BH of the truss shown.
D : SOLID MECHANICS Q. 1 Q. 9 carry one mark each. Q.1 Find the force (in kn) in the member BH of the truss shown. Q.2 Consider the forces of magnitude F acting on the sides of the regular hexagon having
More informationA HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS
A HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS A. Kroker, W. Becker TU Darmstadt, Department of Mechanical Engineering, Chair of Structural Mechanics Hochschulstr. 1, D64289 Darmstadt, Germany kroker@mechanik.tudarmstadt.de,
More informationNORMAL STRESS. The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts.
NORMAL STRESS The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts. σ = force/area = P/A where σ = the normal stress P = the centric
More informationPostBuckling Behavior of Laminated Composite Cylindrical Shells Subjected to Axial, Bending and Torsion Loads
World Journal of Engineering and Technology, 25, 3, 8594 Published Online November 25 in SciRes. http://www.scirp.org/journal/wjet http://dx.doi.org/.4236/wjet.25.349 PostBuckling Behavior of Laminated
More informationThermal buckling and postbuckling of laminated composite plates with. temperature dependent properties by an asymptotic numerical method
hermal buckling and postbuckling of laminated composite plates with temperature dependent properties by an asymptotic numerical method F. Abdoun a,*, L. Azrar a,b, E.M. Daya c a LAMA, Higher School of
More informationN = Shear stress / Shear strain
UNIT  I 1. What is meant by factor of safety? [A/M15] It is the ratio between ultimate stress to the working stress. Factor of safety = Ultimate stress Permissible stress 2. Define Resilience. [A/M15]
More informationITE IMPACT ON. Summary. concurrent. phenomena delamination. subroutine. simulations discussed. Keywords: Volnei Tita.
NUMERICAL AND EXPERIMENTAL ANALYSES OF LOW VELOCITY IMPACT ON THIN COMPOS ITE Marcelo L. Ribeiro Department of Aeronautical Engineeringg Engineering Scholl of São Carlos University of São S Paulo malribei@usp.
More informationGEOMETRIC NONLINEAR ANALYSIS
GEOMETRIC NONLINEAR ANALYSIS The approach for solving problems with geometric nonlinearity is presented. The ESAComp solution relies on Elmer opensource computational tool [1] for multiphysics problems.
More informationAn orthotropic damage model for crash simulation of composites
High Performance Structures and Materials III 511 An orthotropic damage model for crash simulation of composites W. Wang 1, F. H. M. Swartjes 1 & M. D. Gan 1 BU Automotive Centre of Lightweight Structures
More informationCOMPRESSIVE BEHAVIOR OF IMPACT DAMAGED COMPOSITE LAMINATES
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS COMPRESSIVE BEHAVIOR OF IMPACT DAMAGED COMPOSITE LAMINATES Hiroshi Suemasu*, Wataru Sasaki**, Yuuichiro Aoki***, Takashi Ishikawa**** *Department of
More informationCOMPUTATIONAL MODELING APPLIED TO THE STUDY OF THERMAL BUCKLING OF COLUMNS
COMPUTATIONAL MODELING APPLIED TO THE STUDY OF THERMAL BUCKLING OF COLUMNS R. da S. Michaello a, D. Helbig b, L. A. O. Rocha b, M. de V. Real c, E. D. dos Santos c, and L. A. Isoldi c a Universidade Federal
More informationPREDICTION OF BUCKLING AND POSTBUCKLING BEHAVIOUR OF COMPOSITE SHIP PANELS
FONDATĂ 1976 THE ANNALS OF DUNAREA DE JOS UNIVERSITY OF GALATI. FASCICLE IX. METALLURGY AND MATERIALS SCIENCE N 0. 007, ISSN 15 08X PREDICTION OF BUCKLING AND POSTBUCKLING BEHAVIOUR OF COMPOSITE SHIP PANELS
More informationImpact and Crash Modeling of Composite Structures: A Challenge for Damage Mechanics
Impact and Crash Modeling of Composite Structures: A Challenge for Damage Mechanics Dr. A. Johnson DLR Dr. A. K. Pickett ESI GmbH EUROPAM 99 Impact and Crash Modelling of Composite Structures: A Challenge
More informationAnalysis of asymmetric radial deformation in pipe with local wall thinning under internal pressure using strain energy method
Analysis of asymmetric radial deformation in pipe with local wall thinning under internal pressure using strain energy method V.M.F. Nascimento Departameto de ngenharia Mecânica TM, UFF, Rio de Janeiro
More informationKINGS COLLEGE OF ENGINEERING DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK. Subject code/name: ME2254/STRENGTH OF MATERIALS Year/Sem:II / IV
KINGS COLLEGE OF ENGINEERING DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK Subject code/name: ME2254/STRENGTH OF MATERIALS Year/Sem:II / IV UNIT I STRESS, STRAIN DEFORMATION OF SOLIDS PART A (2 MARKS)
More informationBEARING STRENGTH ASSESSMENT OF COMPOSITE MATERIAL THROUGH NUMERICAL MODELS
BEARING STRENGTH ASSESSMENT OF COMPOSITE MATERIAL THROUGH NUMERICAL MODELS Euler S. Dias*, Carlos A. Cimini Jr.* * Federal University of Minas Gerais, Dept. of Structural Engineering, Belo Horizonte 
More informationSIZE EFFECTS IN THE COMPRESSIVE CRUSHING OF HONEYCOMBS
43rd AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Con 2225 April 2002, Denver, Colorado SIZE EFFECTS IN THE COMPRESSIVE CRUSHING OF HONEYCOMBS Erik C. Mellquistand Anthony M.
More informationAn integrated approach to the design of high performance carbon fibre reinforced risers  from micro to macro  scale
An integrated approach to the design of high performance carbon fibre reinforced risers  from micro to macro  scale Angelos Mintzas 1, Steve Hatton 1, Sarinova Simandjuntak 2, Andrew Little 2, Zhongyi
More informationModelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations
Modelling the nonlinear shear stressstrain response of glass fibrereinforced composites. Part II: Model development and finite element simulations W. Van Paepegem *, I. De Baere and J. Degrieck Ghent
More informationA Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber
A Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber Kibong Han Mechatronics Department, Jungwon University, 85 Munmuro, Goesangun, South Korea.
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of Materials Science and Engineering A 6 () 354 doi:.765/663/6..5 D DAVID PUBLISHING Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K * and V V Subba Rao Faculty
More informationNUMERICAL EVALUATION OF THE ROTATIONAL CAPACITY OF STEEL BEAMS AT ELEVATED TEMPERATURES
8 th GRACM International Congress on Computational Mechanics Volos, 12 July 15 July 2015 NUMERICAL EVALUATION OF THE ROTATIONAL CAPACITY OF STEEL BEAMS AT ELEVATED TEMPERATURES Savvas Akritidis, Daphne
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationAdvanced Structural Analysis EGF Cylinders Under Pressure
Advanced Structural Analysis EGF316 4. Cylinders Under Pressure 4.1 Introduction When a cylinder is subjected to pressure, three mutually perpendicular principal stresses will be set up within the walls
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationMECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING
MECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING Steven Roy, Larry Lessard Dept. of Mechanical Engineering, McGill University, Montreal, Québec, Canada ABSTRACT The design and
More informationALGORITHM FOR NONPROPORTIONAL LOADING IN SEQUENTIALLY LINEAR ANALYSIS
9th International Conference on Fracture Mechanics of Concrete and Concrete Structures FraMCoS9 Chenjie Yu, P.C.J. Hoogenboom and J.G. Rots DOI 10.21012/FC9.288 ALGORITHM FOR NONPROPORTIONAL LOADING
More informationPLY WAVINESS ON INPLANE STIFFNESS OF COMPOSITE LAMINATES
PLY WAVINESS ON INPLANE STIFFNESS OF COMPOSITE LAMINATES Cimini Jr., Carlos A., and Tsai, Stephen W. 2 Department of Mechanical Engineering, Federal University of Minas Gerais Av. Antônio Carlos, 6627
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationPrincipal Stresses, Yielding Criteria, wall structures
Principal Stresses, Yielding Criteria, St i thi Stresses in thin wall structures Introduction The most general state of stress at a point may be represented by 6 components, x, y, z τ xy, τ yz, τ zx normal
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationTHE MUTUAL EFFECTS OF SHEAR AND TRANSVERSE DAMAGE IN POLYMERIC COMPOSITES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS THE MUTUAL EFFECTS OF SHEAR AND TRANSVERSE DAMAGE IN POLYMERIC COMPOSITES L.V. Smith 1 *, M. Salavatian 1 1 School of Mechanical and Materials
More informationEffect of loading pulse duration on dynamic buckling of stiffened panels
MAT EC Web of Conferences 16, 76 (214) DOI: 1151/ matecconf/ 21416 76 C Owned by the authors, published by EDP Sciences, 214 Effect of loading pulse duration on dynamic buckling of stiffened panels O Mouhat
More informationTRIALS WITH A SIMPLIFIED METHOD FOR BUCKLING AND ULTIMATE STRENGTH ANALYSIS OF COMPOSITE PLATES
DEPT. OF MATH., UNIVERSITY OF OSLO RESEARCH REPORT IN MECHANICS, No. 1 ISSN 08019940 December 2012 TRIALS WITH A SIMPLIFIED METHOD FOR BUCKLING AND ULTIMATE STRENGTH ANALYSIS OF COMPOSITE PLATES by Qiao
More informationAEROELASTIC ANALYSIS OF SPHERICAL SHELLS
11th World Congress on Computational Mechanics (WCCM XI) 5th European Conference on Computational Mechanics (ECCM V) 6th European Conference on Computational Fluid Dynamics (ECFD VI) E. Oñate, J. Oliver
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationINFLUENCE OF WEB THICKNESS REDUCTION IN THE SHEAR RESISTANCE OF NONPRISMATIC TAPERED PLATE GIRDERS
INFLUENCE OF WEB THICKNESS REDUCTION IN THE SHEAR RESISTANCE OF NONPRISMATIC TAPERED PLATE GIRDERS Paulo J. S. Cruz 1, Lúcio Lourenço 1, Hélder Quintela 2 and Manuel F. Santos 2 1 Department of Civil
More informationEngineering Solid Mechanics
}} Engineering Solid Mechanics 1 (2013) 18 Contents lists available at GrowingScience Engineering Solid Mechanics homepage: www.growingscience.com/esm Impact damage simulation in elastic and viscoelastic
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationNUMERICAL SIMULATION OF DAMAGE IN THERMOPLASTIC COMPOSITE MATERIALS
5 th European LSDYNA Users Conference Composites NUMERICAL SIMULATION OF DAMAGE IN THERMOPLASTIC COMPOSITE MATERIALS Kevin Brown 1, Richard Brooks, Nicholas Warrior School of Mechanical, Materials and
More informationNONLINEAR LOCAL BENDING RESPONSE AND BULGING FACTORS FOR LONGITUDINAL AND CIRCUMFERENTIAL CRACKS IN PRESSURIZED CYLINDRICAL SHELLS
NONINEAR OA BENDING RESPONSE AND BUGING FATORS FOR ONGITUDINA AND IRUMFERENTIA RAKS IN PRESSURIZED YINDRIA SHES Richard D. Young, * heryl A. Rose, * and James H. Starnes, Jr. NASA angley Research enter
More informationNumerical Analysis of Delamination Buckling in Composite Cylindrical Shell under Uniform External Pressure: Cohesive Element Method
Journal of Modern Processes in Manufacturing and Production, Vol. 6, No. 3, Summer 2017 Numerical Analysis of Delamination Buckling in Composite Cylindrical Shell under Uniform External Pressure: Cohesive
More informationTheory at a Glance (for IES, GATE, PSU)
1. Stress and Strain Theory at a Glance (for IES, GATE, PSU) 1.1 Stress () When a material is subjected to an external force, a resisting force is set up within the component. The internal resistance force
More informationMechanics of Materials II. Chapter III. A review of the fundamental formulation of stress, strain, and deflection
Mechanics of Materials II Chapter III A review of the fundamental formulation of stress, strain, and deflection Outline Introduction Assumtions and limitations Axial loading Torsion of circular shafts
More informationCalibration and Experimental Validation of LSDYNA Composite Material Models by Multi Objective Optimization Techniques
9 th International LSDYNA Users Conference Optimization Calibration and Experimental Validation of LSDYNA Composite Material Models by Multi Objective Optimization Techniques Stefano Magistrali*, Marco
More informationPREDICTION OF FAILURE BEHAVIOUR OF COMPOSITE LATTICE STRUCTURE UNDER COMPRESSIVE LOAD
PREDICTION OF FAILURE BEHAVIOUR OF COMPOSITE LATTICE STRUCTURE UNDER COMPRESSIVE LOAD MinHyeok Jeon. 1, MinSong Kang 1, MunGuk Kim 1, EunSu Go 1, InGul Kim. 1, and SangWoo Lee 2 1 Aerospace Engineering,
More information2766. Differential quadrature method (DQM) for studying initial imperfection effects and pre and postbuckling vibration of plates
2766. Differential quadrature method (DQM) for studying initial imperfection effects and pre and postbuckling vibration of plates Hesam Makvandi 1, Shapour Moradi 2, Davood Poorveis 3, Kourosh Heidari
More informationProbabilistic Assessment of a Stiffened Carbon Fibre Composite Panel Operating in its Postbuckled Region Authors: Correspondence:
Probabilistic Assessment of a Stiffened Carbon Fibre Composite Panel Operating in its Postbuckled Region Authors: D. Elder and R. Thomson Cooperative Research Centre for Advanced Composite Structures Limited
More informationAE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF HOOP STRESSES FOR A THINWALL PRESSURE VESSEL
Objective AE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF OOP STRESSES FOR A TINWA PRESSURE VESSE This experiment will allow you to investigate hoop and axial stress/strain relations
More informationCOROTATIONAL NONLINEAR DYNAMIC ANALYSIS OF LAMINATED COMPOSITE SHELL STRUCTURES
Copyright c 009 by ABCM January 0408, 010, Foz do Iguaçu, PR, Brazil COROTATIONAL NONLINEAR DYNAMIC ANALYSIS OF LAMINATED COMPOSITE SHELL STRUCTURES Felipe Schaedler de Almeida, schaedleralmeida@gmail.com
More informationPostbuckling Analyses of Elastic Cylindrical Shells under Axial Compression
Postbuckling Analyses of Elastic Cylindrical Shells under Axial Compression Takaya Kobayashi and Yasuko Mihara Mechanical Design & Analysis Corporation Tokyo, Japan Abstract: In the design of a modern
More information6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS
6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS Blondet et al. [25] carried out a cyclic test on an adobe wall to reproduce its seismic response and damage pattern under inplane loads. The displacement
More informationFINITE ELEMENT AND EXPERIMENTAL STUDY OF NOVEL CONCEPT OF 3D FIBRE CELL STRUCTURE
FINITE ELEMENT AND EXPERIMENTAL STUDY OF NOVEL CONCEPT OF 3D FIBRE CELL STRUCTURE M. Růžička, V. Kulíšek 2, J. Had, O. Prejzek Department of Mechanics, Biomechanics and Mechatronics, Faculty of Mechanical
More informationMODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE
MODELING OF THE BEHAVIOR OF WOVEN LAMINATED COMPOSITES UNTIL RUPTURE Jean Paul Charles, Christian Hochard,3, Pierre Antoine Aubourg,3 Eurocopter, 375 Marignane cedex, France Unimeca, 6 rue J. Curie, 3453
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationCHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES
CHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES * Governing equations in beam and plate bending ** Solution by superposition 1.1 From Beam Bending to Plate Bending 1.2 Governing Equations For Symmetric
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationCOMPARISON OF COHESIVE ZONE MODELS USED TO PREDICT DELAMINATION INITIATED FROM FREEEDGES : VALIDATION AGAINST EXPERIMENTAL RESULTS
COMPARISON OF COHESIVE ZONE MODELS USED TO PREDICT DELAMINATION INITIATED FROM FREEEDGES : VALIDATION AGAINST EXPERIMENTAL RESULTS A. Uguen 1, L. Zubillaga 2, A. Turon 3, N. Carrère 1 1 Laboratoire Brestois
More information